- Open Access
Drug delivery applications of poly-γ-glutamic acid
Future Journal of Pharmaceutical Sciences volume 7, Article number: 125 (2021)
Poly-γ-glutamic acid (γ-PGA) is a biopolymer of microbial origin, consisting of repeating units of l-glutamic acid and/or D-glutamic acid. The biopolymer has found use in the fields of agriculture, food, wastewater, and medicine, owing to its non-toxic, biodegradable, and biocompatible properties. Due to its biodegradability, γ-PGA is being tipped to dislodge synthetic plastics in drug delivery application. High cost of production, relative to plastics, is however a clog in the wheel of achieving this.
Main body of abstract
This review looked at the production, nanoparticles fabrication, and drug delivery application of γ-PGA. γ-PGA production optimization by modifying the fermentation medium to tailor towards the production of desirable polymer at reduced cost and techniques for the formulation of γ-PGA nanoparticle as well as its characterization were discussed. This review also evaluated the application of γ-PGA and its nanoparticles in the delivery of drugs to action site. Characterization of γ-PGA and its nanoparticles is a crucial step towards determining the applicability of the biopolymer. γ-PGA has been used in the delivery of active agents to action sites.
This review highlights some of the efforts that have been made in the appraisal of γ-PGA and its nanoparticles for drug delivery. γ-PGA is a candidate for future extensive use in drug delivery.
Polyglutamic acid (PGA) is a polymer of repeating units of glutamic acid. The repeating units can be l-glutamic acid and/or D-glutamic acid. There are two isoforms of polyglutamic acid: α-PGA and γ-PGA. The classification is based on whether the carboxyl group is attached through α or γ-linkages. In poly-γ-glutamic acid (γ-PGA) structure (Fig. 1), amide linkages with the monomers exist between α-amino and γ-carboxyl functional groups . γ-PGA is a non-immunogenic, biodegradable anionic homo-polyamide . Bacterial production of α-PGA is tasking and is only achievable with recombinant technology , whereas γ-PGA is produced by gram-positive bacteria, chiefly Bacillus sp.  and some gram-negative bacteria like Fusobacterium nucleatum . Compared with γ-PGA produced by bacteria, α-PGA synthetically produced has a lower molecular mass (<10kDa) which limits its application. The molecular mass of γ-PGA is higher and commonly varies between ~ 100 and >1000 kDa .
The production cost of pure microbial γ-PGA is a major impediment to the widespread industrial use of the biopolymer. Many types of researches, as a result, have focused on optimizing the growth condition of the producing bacteria, with a view to obtaining high yield and desirable molecular mass at a cheaper cost . γ-PGA production and its properties depend largely on the nutrient composition of the fermentation medium as well as the pH of the medium, temperature and period of incubation, and the producing microbe .
The hydrophilicity, biodegradability, and biocompatibility of γ-PGA make it a suitable candidate for drug delivery . A loose α-carboxyl group, which confers hydrophilicity, is present on every glutamate unit of the biopolymer . The hydrophilicity was exploited to improve the water solubility of paclitaxel in a conjugate of the drug with γ-PGA . The presence of carboxyl groups in the structure of γ-PGA (Fig. 1) also makes the biopolymer amenable to modification, by undergoing ionic interaction with cationic active agents or polymer, to form a stable complex . The negative charge on the anionic γ-PGA has been exploited to form a nanoparticle complex with positively charged chitosan  and polymer-drug complex with doxorubicin . γ-PGA can assume a number of conformations, depending on the pH of the solution and polymer concentration . There are strong intramolecular hydrogen bonds between the monomer units of the biopolymer in an unionized state . These hydrogen bonding are shown by Ho et al. , using optical rotatory dispersion, to be responsible for the stacked α-helix conformation of free γ-PGA (in aqueous solution) that led to hydrophobicity at pH 2 (unionized). The conformation reportedly changed at pH 4.09 due to a breakup of the bonding, which resulted in 50% of the earlier conformation changing into a random-coil conformation. At pH higher than 6.5 however, γ-PGA existed in a complete linear random-coil conformation . At this conformation, γ-PGA offers multiple binding sites to cationic molecules .
Esterification is a desirable method of modifying γ-PGA to allow for the delivery of poorly water-soluble agents . Hydrophobic modification with different esters retains the intramolecular hydrogen bonding stabilized α-helix structure of γ-PGA. This conformation opens up the structure and optimizes electrostatic interaction between γ-PGA and positively charged functional groups, with minimal repulsive effect on like ions .
A self-assembled nanoparticulate system of hydrophobically modified γ-PGA with l-phenylalanine ethyl ester was developed by Akagi et al. . The nanoparticle reportedly consists of a l-phenylalanine ethyl ester hydrophobic core and γ-PGA hydrophilic shell. This modification enhanced the loading and stability of the poorly water-soluble antimalarial, quinine . Hydrophobic derivatives such as benzylamidated γ-PGA  are capable of assuming a stable helix structure with orderly arranged side chains on the outer edge, resulting in a rigid conformation [16, 19, 20]. The orderly alignment spurs a strong π-π stacking interaction between the benzyl groups of the derivative . The π-π stacking interaction results in higher drug loading efficiency of a drug, gambogic acid, with a conjugated system .
In this review, we give an insight into the optimization of fermentation medium for γ-PGA synthesis, formulation and characterization of γ-PGA and nanoparticles, and the potential application of the biopolymer in drug delivery.
l-Glutamic acid serves as the precursor for microbial production of γ-PGA. It can be incorporated into the biosynthetic pathway endogenously or exogenously . One of the steps involved in γ-PGA biosynthesis is racemization. This ensures the incorporation of D-glutamic acid (by converting the l-enantiomer supplied exo- or endogenously) into the evolving γ-PGA chain . Ashiuchi et al. [23, 24] reported a homologous pair of glutamate racemase gene (race/glr and yrpC) in Bacillus subtilis. The glr is an essential gene for l-glutamate conversion into D-glutamate during γ-PGA biosynthesis in B. subtilis .
ATP is said to be the catalyst for the polymerization of PGA. The encoded gene, pgsBCA, on polyglutamate synthase (pgs) was also reported to be the lone architect of γ-PGA polymerization . The two-part system of DegS-DegU, DegQ, and SwrA, as well as the ComP-ComA system, is thought to be responsible for the regulation of γ-PGA synthesis [27, 28] (Fig. 2).
Exo-γ-glutamyl peptidase and endo-γ-glutamyl peptidase were the enzymes identified as having the potential to degrade γ-PGA in Bacilli .
γ-PGA production and medium optimization
The major impediment to the widespread industrial application of pure microbial γ-PGA is the production cost. Researchers have, therefore, focused on reducing this cost by utilizing cheap and renewable substrates as well as optimizing the growth condition of the producing bacteria with a view to obtaining high yield and desirable molecular mass .
γ-PGA production using cheap and renewable substrate
Odeniyi and Avoseh  investigated the production of γ-PGA using agricultural residue as substrate. The best producing bacteria, isolated from decomposing Coix lacryma-jobi, was identified as Bacillus toyonensis As8. The highest γ-PGA yield of all the agricultural residue studied (sorghum leaves, corn cob, rice bran, Coix noir leaves, and cassava peel) was reported to be from cassava peel, used at 20g/l in the fermentation medium.
In a similar work, corn starch (CS) and soybean meal (SBM) were employed as solid substrate in the synthesis of γ-PGA by Bacillus amyloliquefaciens JX-6 . The output between sterilized and non-sterilized fermentation medium was compared. Industrial monosodium glutamate (IMSG) was employed in the medium as a γ-PGA precursor. Response surface methodology (RSM) showed the final components of the medium SBM, CS, and IMSG to be in the ratio 5:5:1 . The reported yield for sterilized and non-sterilized solid-state fermentation were 166.99 ± 1.94g/kg and 134.25 ± 4.38g/kg respectively. The authors opined that, although the sterilized fermentation produced a higher γ-PGA yield, non-sterilized fermentation could reasonably reduce the fermentation time and consequently the cost of production.
Mohanraj et al.  compared γ-PGA production by B. subtilis 2756 using soybean and sago as substrates in both glutamate-dependent and non-dependent fermentation media. The substrates were used at 90 g/l for the glutamate-dependent media and 75 g/l for glutamate independent. RSM was used to optimize the concentration of L-glutamic acid, NaCl, and yeast extract contents of the media. The optimized media resulted in an approximately 7% increase in γ-PGA production . γ-PGA was said to be produced by the organism in both glutamate- and non-glutamate-dependent media. A higher yield was, however, reported in the glutamate containing medium.
Fishmeal wastewater was employed as the source of nitrogen for γ-PGA synthesis by Bacillus subtilis A3 . The fermentation medium contained 30 g/l glucose, 15 g/l chemical oxygen demand (COD) of fishmeal wastewater, and 25 g/l L-glutamate. Used alone as fermentation medium, fishmeal wastewater yielded a small amount of γ-PGA which suggested the ability of B. subtilis A3 to produce the polymer using fishmeal wastewater . Compared with different sources of nitrogen which included tryptone, peptone, yeast extract, maize flour, fish protein ammonium sulphate, and soy bean, it was reported that only tryptone (29 ± 0.30 g/l) and fish protein (27.05 ± 0.12 g/l) had a greater influence on the yield than fishmeal wastewater (25.01 ± 0.32 g/l).
Optimization of medium composition
Composition of the fermentation medium is one of the most important determinants of both the production rate as well as the properties of γ-PGA produced by microbial fermentation . The effect of medium composition was shown by Birrer et al.  when the medium NaCl concentration was varied. The molecular mass of the γ-PGA synthesized by Bacillus licheniformis ATCC 9945a changed from 1200 to 2200 kDa when the concentration of NaCl was increased from 0 to 4%.
Bajaj et al.  obtained an improved γ-PGA production of 26.12 g/l by B. licheniformis NCIM 2324 (from 5.27 g/l for basal medium) from optimized medium. The optimum medium, obtained by RSM, contained 62.4 g/l glycerol, 15.2 g/l citric acid, 8.0 g/l ammonium sulphate, and 20 g/l L-glutamic acid. Further optimization was carried out in which metabolic precursors for γ-PGA production, L-glutamine (0.07 g/l), and -ketoglutaric acid (1.46 g/l) were added to the fermentation medium . The improved γ-PGA yield of 35.75 g/l (compared to the 26.12 g/l) was opined to be due to a better L-glutamic acid utilization caused by the added metabolic precursor.
Culture medium volume and yeast extract proportion are determining factors for γ-PGA production in B. licheniformis A13, a glutamate-independent γ-PGA producer . The optimum medium designed by Plackett-Burman produced γ-PGA of 28.2 g/l after 72 h. The medium composed of 50 g/l glucose, 2 g/l yeast extract, 3 g/l NH4Cl, 0.006 g/l FeSO4.4H2O, 6.4 g/l K2HPO4, 0.8 g/l MgSO4.7H2O, 0.00084 g/l CaCl2.2H2O, 0.8 g/l NaCl, and 0.1 ml solution of trace elements. The volume of the culture medium was 25 ml .
A higher yield of γ-PGA with optimized medium containing 30 g/l L-glutamate, 40 g/l yeast extract, and 20 g/l glucose with B. subtilis ZJU-7 as the producer was reported . The concentration of the glucose in the medium was maintained within the range 3–10 g/l by the fed-batch method. γ-PGA production up to 101.1 g/l, representing up to 3.2-fold increase in comparison to the batch fermentation, was reported.
The effect of amino acids addition to a fermentation medium of B. subtilis Z15 has been demonstrated . Increase in γ-PGA yield corresponding to 23.18%, 12.15%, and 31.46% was reported on the respective addition of 3 g/l aspartic acid (at 0 h), 1.5 g/l phenylalanine (at 0 h), and 7 g/l glutamic acid (at 24 h). It was reported that crude extract of glutamic acid after isoelectric crystallization (CEGA) could also be used in place of glutamate for the production of γ-PGA. The optimized amino acid content, arrived at using response surface methodology, contained 9 g/l CEGA, 4g/L aspartic acid, and 1.55 g/L phenylalanine. A yield 63.1% higher than control was reported when the medium was applied in 5-L bioreactor.
Culture condition optimization
Another crucial factor in γ-PGA production is the culture pH . Optimum γ-PGA yield was reported for B. licheniformis ATCC 9945A at pH 6.5 . This was however achieved with B. subtilis IFO 3335 at a pH of 7 .
Wu et al.  proposed a process for optimizing glutamate utilization and γ-PGA yield. In the process, the pH of the fermentation medium was sustained at 7 for 24 h to enhance maximal biomass accumulation. The pH was then lowered and maintained at 6.5 for optimal glutamate utilization and consequent γ-PGA yield. This process increased both glutamate utilization and γ-PGA yield from 24.3 to 29.3 g/l and 22.2 to 27.7 g/l respectively .
A procedure aimed at reducing the cost of production of γ-PGA by avoiding exogenous addition of L-glutamic acid was developed . This was achieved by co-culturing L-glutamate-dependent B. subtilis with Corynebacterium glutamicum and utilizing glucose and sucrose as carbon sources. The fermentation time was also reduced by the process. The average molecular mass of the produced γ-PGA was reported to be 1240 kDa.
The recovery of peptidoglycan bound γ-PGA, as in Bacillus anthracis, is difficult to achieve because the polymer is not released into the medium. B. anthracis is also known to be toxic, which makes its industrial application untenable . γ-PGA secreted into the medium can be recovered by three methods: precipitation by reducing water solubility, precipitation by complex formation, and filtration . Removal of the microbial biomass is the first step in any of these recovery methods. The biomass is removed by centrifugation or filtration using a 0.45-μm filter . The water solubility of γ-PGA can be reduced by adding ethanol to the supernatant or filtrate from the fermentation medium. This brings about the precipitation of the γ-PGA from solution . This procedure however does not guarantee a pure γ-PGA production due to the fact that proteins and polysaccharides in solution can be co-precipitated with the biopolymer . Precipitation by complex formation involves the use of metals for a complexation reaction with γ-PGA in solution. Commonly used metals include Al3+, Fe3+, Cu2+, and Cr3+ . The molecular size of high molecular weight γ-PGA differs from the remaining components of the medium. A series of filtration and buffer exchange steps capitalize on this difference to effect γ-PGA separation .
Characterization of γ-PGA
Characterization of γ-PGA is an important step towards the determination of areas to which the polymer can be applied. Some techniques are available for the analysis and characterization of γ-PGA.
Fourier-transform infrared (FTIR) spectroscopy is used for the polymer’s identification. The spectra indicate specific functional groups/bonds in the polymer. Ho et al.  reported γ-PGA in KBr pellet to indicate the following: a weak C=O absorption at ~1394–1454 cm−1, a characteristic strong amide and C-N groups absorptions at ~1620–1655 cm−1 and 1085–1165 cm−1 respectively, a strong hydroxyl absorption at around 3400–3450 cm1, characteristic aliphatic N-H stretching between 2900 and 2800 cm−1, and 1600–1660 cm−1 and 1390–1450 cm−1 for amide and C=O groups respectively.
Nuclear magnetic resonance (NMR)
The degree of esterification and homogeneity of γ-PGA are usually determined using 1H and 13C-NMR .
Amino acid analysis
This analysis intends to evaluate the purity of the synthesized γ-PGA. The TLC detection of only glutamic acid is an attestation to the purity of the polymer . The step involves the acid hydrolysis of γ-PGA using 6M HCl at 100 °C for specific hours in a glass vial. The hydrolyzed polymer is dried by evaporating the remnant HCl. The product, after drying, is dissolved in water and the amino acid content TLC-analyzed . Goto and Kunioka  analyzed γ-PGA using an amino acid autoanalyzer. The hydrolysis was done using 6N HCl at 150 °C for 3 h in an enclosed glass tube under a nitrogen ambience using a Pico-Tag apparatus.
Molecular mass determination
The properties and eventual fields of application of γ-PGA are determined by the molecular mass of the polymer . Molecular mass of γ-PGA is often measured by gel permeation chromatography (GPC). The molecular mass is determined by calibrating against particular standards . Molecular mass of γ-PGA was determined using GPC . The concentration of the sample used was 1 mg/mL (200 μL volume injected) and 50 mM aqueous solution of NaCl to acetonitrile (4:1) employed as eluant. The rate of flow of the eluant was 0.7 mL/min. Calibration curve to determine molecular mass was made using poly-(styrene sulfonic acid, sodium salt) as standard. There is often the need for molecular mass reduction of γ-PGA intended for drug delivery application. Techniques used for molecular mass reduction include medium composition alteration, ultrasonic degradation, alkaline hydrolysis, and microbial or enzymatic degradation .
Formulation of γ-PGA Nanoparticles
Nanoparticles (NPs) have gained tremendous attention in drug delivery system over the years. This is due to their biocompatibility with body cells, low toxicity, and also their ability for controlled release . Nanoparticles, in addition to the ability to sustain drug release at the site of action, enjoy high intracellular uptake and also the capability of improving drug stability . Nanoparticles can be nanocapsules, in which the active agent is contained within an oily reservoir core surrounded by a membrane wall. They can also be nanospheres in which the agent is dispersed in a matrix of the particles .
The delivery system also ensures controlled drug release, bioavailability, and retention in site of action [54, 55]. Factors such as solubility of the active agent, molecular weight, biodegradability, surface charge, size requirement, biocompatibility, and type of polymeric system determine the method of choice for nanoparticles preparation . Formulation of γ-PGA as nanoparticles for drug delivery offers a number of merits which include improved drug stability, high drug loading efficiency, and the possibility of drug incorporation without the need for a chemical reaction .
Solvent exchange method
γ-PGA nanoparticle formulation using solvent exchange was described by Matsusaki et al. . γ-PGA was the hydrophilic portion while l-phenylalanine ethyl ester or l-leucine methyl ester served as the hydrophobic side. The amphiphilic derivatives of γ-PGA, Phe-γ-PGA and Leu-γ-PGA, were made by dissolving 4.7 unit mmol γ-PGA in an aqueous solution of 0.3N NaHCO3. Carbodiimide, phenylalanine, and leucine were added to the solution in sufficient quantity and then agitated for a period of 30 min at 4 °C. The consequent solution was kept at a room temperature condition for 24 h, thereafter dialyzed, and the derivatives retrieved after 72 h of freeze-drying. Self-assembled nanoparticles were then made by dissolving 10 mg of Leu-γ-PGA and Phe-γ-PGA in a mixture of equal volume of DMSO and distilled water. This was followed by dialysis and lyophilization. Phe-γ-PGA with conversion degrees of 42 and 58 yielded nanospheres of approximately 200 nm (characterized by TEM) .
Ionic gelation method
This method involves the interaction between the surface charges of a polymer and another polymer of opposite charge or a polycation or polyanion . A nanoparticle of γ-PGA and chitosan was prepared by Lin et al.  using this technique. The nanoparticles were used to deliver oral insulin. In the preparation, 2 mL of a 1mg/ml γ-PGA (pH 7.4) aqueous solution was flushed through a pipette into aqueous chitosan under magnetic stirring. The formed nanoparticles were removed by ultracentrifugation (32,000 rpm for 50 min). The diameters of the NPs were reported to fall between 110 and 150 nm. The zeta potential of the formed NPs depended on the amount of negatively charged γ-PGA and positively charged chitosan used in the preparation .
Characterization of γ-PGA nanoparticles
Characterization of nanoparticles is very crucial to understanding the behavior of formulated NPs in order to channel to appropriate application. NP size and size distribution affect important parameters such as drug release, stability, cellular uptake, and tissue penetration . Smaller particles, compared to larger ones, possess a larger surface area but lower drug encapsulation ability. The encapsulated drugs are released faster during degradation because of nearness to the NP surface . Smaller particles however default in stability because of being prone to aggregation . There is thus the need for a balance between what are large and what are small particles.
Particle size and size distribution of γ-PGA NPs are determined by dynamic light scattering (DLS) and photon correlation microscopy, scanning electron microscopy (SEM), atomic force microscopy (AFM), and transmission electron microscopy (TEM) [61, 62].
The surface charge and the surface hydrophobicity are determinants in the interaction of NPs with biological environment. The zeta potential, determined by a zetasizer, is a function of the surface on the NPs. The values can either be negative or positive, depending on the materials making up the particles . Effect of pH on the zeta potential of curcumin-loaded 6-deoxy-6-arginine modified chitosan (DC)/γ-PGA nanoparticles was reported by Su et al. . The charge on DC reportedly increased from +46.6 to +28.8 mV as the pH was raised from 4 to 9. The same pH change resulted in a decrease in the charge on γ-PGA from − 26.2 to − 38.6 mV. The NPs were prepared at an optimum pH of 6, in which interaction between γ-PGA and DC was strongest.
Application of poly-γ-glutamic acid in drug delivery
γ-PGA has been used in several fields of endeavor. The wide application is owed to its unique characteristics. Its properties which include water solubility, non-toxicity, biodegradability, and biocompatibility have endeared the microbial polymer to many fields of application . γ-PGA has been utilized for the delivery of some category of drugs (Fig. 3) [12, 18, 22, 64,65,66,67,68,69].
Anticancer delivery application
The molecular mass of γ-PGA is crucial to drug delivery as well as the ability to control drug release. Li et al.  reported molecular masses between 3 × 104 and 6 × 104 as necessary for conjugation with the anticancer agent, paclitaxel. The conjugate offered a water-soluble derivative of paclitaxel. Apart from this, the conjugate was shown to display a superior therapeutic index, compared to paclitaxel. There was a disappearance of established breast and ovarian cancers within 2 weeks upon injection of the conjugate at a dose equivalent to 40 mg/kg and 160 mg/kg of paclitaxel respectively. The remarkable antitumor activity of the conjugate was due to a greater uptake by the tumor cells, compared to free paclitaxel. Unlike paclitaxel also, the γ-PGA-paclitaxel conjugate exhibited negligible tubulin polymerization activity and did not enhance paclitaxel-dependent CHO mutant cell line growth .
Paclitaxel poliglumex, a macromolecular taxane formulated by conjugation between paclitaxel and γ-PGA, was designed by Singer . The conjugate offered a water-soluble alternative to paclitaxel, in addition to an improved pharmacokinetic profile, ensured a longer drug exposure to the tumor cells and minimized systemic exposure. Animal study demonstrated the conjugate to be of higher efficacy and lesser untoward effect, compared to standard paclitaxel .
The eligibility of γ-PGA as a vector for the controlled release of anticancer drug, doxorubicin, was evaluated by Manocha and Margaritis . The formulation was made by ionic complexation of the anionic γ-PGA and cationic doxorubicin (DOX). The efficiency of complexation between the drug and the polymer was almost 100%. A pH-dependent in vitro drug release from the complex was reported. Up to 40% burst release of doxorubicin from the complex (in the first 8 h) was observed at pH 2.2. The burst was followed by a slow release over 7 days. The burst was, however, not observed at a pH of more than 2.2. A controlled release of doxorubicin over time is thus achievable with a pH-triggered DOX/γ-PGA complex .
Ye et al.  formulated a cisplatin-attached γ-PGA. The conjugate produced a water-soluble derivative of cisplatin with molecular weight of conjugation being between 4.5 and 6.0 × 104 Da. An initial burst release of cisplatin from the conjugate (in PBS) within the first 6 h, followed by a subsequent sustained release, was reported. Although less potent than free cisplatin against breast cancer Bcap-37 cell line growth in vitro, γ-PGA-cisplatin conjugate injected as 3 doses (with a 2-day interval between doses) reportedly displayed a greater antitumor activity and lesser toxicity in vivo. Bodyweight loss in the mice treated with free cisplatin was not observed with the conjugate .
A novel nanoparticle carrier to evaluate curcumin delivery was designed by Su et al. . The nanoparticles were prepared by ionic interaction between 6-deoxy-6-arginine-modified chitosan and γ-PGA. The encapsulation efficiency and drug loading capacity reported were 79.5% and 11.31% respectively. The formulation was also said to be stable at temperatures, 30–60 °C and pH 3–9. Drug release from the nanoparticles was evaluated in simulated gastric and intestinal fluids, and compared with the release of curcumin from ethanol. In the simulated gastric fluid (SG), a burst release (within 30 min) from ethanol and NPs were respectively 38.95 and 12.77%. A total release (in SG) of 69.75% and 31.85% occurred for free curcumin and NPs respectively. Upon incubation in the simulated intestinal fluid (SI), free curcumin was slowly released continuously. A more rapid release was reported for curcumin-loaded NP (from 2 to 4 h), compared with in SG, which resulted in a more significant release at the intestinal pH.
A NP delivery system for the controlled delivery of doxorubicin to tumor cells was designed . The nanoparticle system composed of γ-PGA, graphene oxide (GO), and chitosan oligosaccharide (CO). Graphene oxide was linked covalently with chitosan oligosaccharide and γ-PGA loaded onto the composite to form GO-CO-γ-PGA system. Controlled and sustained release of doxorubicin loaded on the nanocarrier were reported. An in vitro cytotoxicity assay, using MTT, had GO-CO-γ-PGA-DOX display higher efficacy in proliferation inhibition than when γ-PGA was absent in the system .
Benzylamidated γ-PGA derivative was used as the drug loading core in a drug delivery system for the natural anticancer, gambogic acid . The outer shell consisted of an amphiphilic hyaluronic acid derivative grafted with all-trans retinoic acid. The drug was incorporated into the benzylamidated γ-PGA via a π-π stacking interaction . An encapsulation efficiency of almost 100% was reported at a drug-polymer ratio of less than 10%. The system also offered a tumor targeting property and an enhanced circulation time. The π-π stacking and hydrophobic interaction with respect to encapsulation efficiency was compared, which depicted a drastic reduction in encapsulation efficiency when benzylamidated γ-PGA was substituted with propylated γ-PGA derivative .
Antimicrobial delivery application
γ-PGA was shown to reduce the toxic effect of amphotericin B while retaining the antifungal activity . Zia et al.  investigated the ability of γ-PGA NPs to ferry the antifungal, amphotericin B. The in vitro antifungal activity of the γ-PGA-based NP formulation against Candida albicans was studied. The formulation was compared with Fungizone®, a marketed brand of amphotericin B. Antifungal activity of the γ-PGA-based NP was comparable to Fungizone® but the NP formulation showed reduced toxicity to erythrocyte and also had an insignificant effect on mammalian cell viability  (Table 1).
γ-PGA was hydrophobically modified to enhance the stability and bioavailability of quinine . An amphiphilic polymer was formed with l-phenylalanine ethyl ester as the hydrophobic core. A stable nanodispersion of quinine was formed with the amphiphilic polymer acting as a surfactant. Bioavailability of quinine following this formulation reportedly increased by up to 6.5 folds.
Delivery of oral insulin
The conventional subcutaneous insulin administration causes poor patient compliance and glucose control [70, 71]. Oral insulin administration offers a better ground as the insulin transits the portal circulation and through the liver into the systemic circulation, which mimics physiological insulin . Sonaje et al.  formulated a γ-PGA-based nanoparticle system with chitosan as a copolymer in the formulation. The insulin incorporated nanoparticle was pH-dependent and prepared by an ionic gelation method. To prevent insulin degradation in the stomach, the freeze-dried nanoparticle was reportedly protected with an enteric-coated capsule. The result of an in vivo dissolution test indicated the stability of the nanoparticle in the low pH gastric environment but was readily released in the small intestine. Relative bioavailability of insulin was 20% which indicated the ability of the formulation to deliver insulin orally .
The application of γ-PGA in drug delivery is on the rise, owing to their tremendous qualities. These qualities include non-toxicity, water solubility, biodegradability, and biocompatibility. The presence of a free α-carboxyl group on the monomer units of γ-PGA presents points of coupling with other polymers or active agent. The ability to form a self-assembled amphiphilic nanoparticle with hydrophobic esters give the biopolymer an added edge for the delivery of poorly water-soluble agents. γ-PGA has been formulated as nanoparticles to exploit the additionally incredible characteristics offered by nanoscale sized system such as high drug encapsulation efficiency, improved stability, solubility and controlled release.
Availability of data and materials
All data and material available on request.
Industrial monosodium glutamate
Response surface methodology
Chemical oxygen demand
Crude extract of glutamic acid
Nuclear magnetic resonance
Thin layer chromatography
Gel permeation chromatography
Transmission electron microscopy
Phosphate buffer saline
Dynamic light scattering
Scanning electron microscopy
Atomic force microscopy
Chinese hamster ovary
6-Deoxy-6-arginine modified chitosan
Simulated gastric fluid
Simulated intestinal fluid
Shih L, Van YT (2001) The production of poly-(γ-glutamic acid) from microorganisms and its various applications. Bioresour Technol 79(3):207–225. https://doi.org/10.1016/S0960-8524(01)00074-8
Buescher JM, Margaritis A (2007) Microbial biosynthesis of polyglutamic acid biopolymer and applications in the biopharmaceutical, biomedical and food industries. Crit Rev Biotechnol 27(1):1–19. https://doi.org/10.1080/07388550601166458
Ogunleye A, Bhat A, Irorere VU, Hill D, Williams C, Radecka I (2015) Poly-γ-glutamic acid: production, properties and applications. Microbiology 161(1):1–17. https://doi.org/10.1099/mic.0.081448-0
Candela T, Moya M, Haustant M, Fouet A (2009) Fusobacterium nucleatum, the first Gram-negative bacterium demonstrated to produce polyglutamate. Can J Microbiol 55(5):627–632. https://doi.org/10.1139/W09-003
Richard A, Margaritis A (2003) Rheology, oxygen transfer, and molecular weight characteristics of poly(glutamic acid) fermentation by Bacillus subtilis. Biotechnol Bioeng 82(3):299–305. https://doi.org/10.1002/bit.10568
Kumar MMM, Xavier JR, Gopalan N (2018) Poly (γ-) Glutamic acid: a promising biopolymer. Def Life Sci J 3(3):301–306. https://doi.org/10.14429/dlsj.3.12192
Wang Q, Wei X, Chen S (2017) Production and application of poly-γ-glutamic acid. In: Current Developments in Biotechnology and Bioengineering. Elsevier, pp 693–717
Anju AJ, Binod P (2016) Synthesis of multifunctional γ-PGA-based superparamagnetic iron oxide nanoparticles for magnetic resonance imaging and controlled drug release. Biologia 71(9):967–971. https://doi.org/10.1515/biolog-2016-0130
Li C, Yu DF, Newman RA, Cabral F, Stephens LC, Hunter N, Milas L, Wallace S (1998) Complete regression of well-established tumors using a novel water-soluble poly(L-glutamic acid)–paclitaxel conjugate. Cancer Res 58(11):2404–2409
Vishweshwar P, McMahon JA, Bis JA, Zaworotko MJ (2006) Pharmaceutical co-crystals. J Pharm Sci 95(3):499–516. https://doi.org/10.1002/jps.20578
Lin YH, Mi FL, Chen CT, Chang WC, Peng SF, Liang HF, Sung HW (2007) Preparation and characterization of nanoparticles shelled with chitosan for oral insulin delivery. Biomacromolecules 8(1):146–152. https://doi.org/10.1021/bm0607776
Manocha B, Margaritis A (2010) Controlled release of doxorubicin from doxorubicin/γ-polyglutamic acid ionic complex. J Nanomater 2010:1–9. https://doi.org/10.1155/2010/780171
He LM, Neu MP, Vanderberg LA (2000) Bacillus lichenformis γ-glutamyl exopolymer: physicochemical characterization and U (VI) interaction. Environ Sci Technol 34(9):1694–1701. https://doi.org/10.1021/es991119e
Zanuy D, Alemán C, Muñoz-Guerra S (1998) On the helical conformation of un-ionized poly (γ-d-glutamic acid). Int J Biol Macromol 23(3):175–184. https://doi.org/10.1016/S0141-8130(98)00047-6
Ho GH, Ho TI, Hsieh KH, Su YC, Lin PY, Yang J, Yang KH, Yang SC (2006) γ-Polyglutamic acid produced by Bacillus subtilis (natto): structural characteristics, chemical properties and biological functionalities. J Chin Chem Soc 53(6):1363–1384. https://doi.org/10.1002/jccs.200600182
Melis J, Zanuy D, Alemán C, García-Alvarez M, Muñoz-Guerra S (2002) On the crystal structure of poly (α-benzyl γ, DL-glutamate) of microbial origin. Macromolecules 35(23):8774–8780. https://doi.org/10.1021/ma020728v
Akagi T, Kaneko T, Kida T, Akashi M (2005) Preparation and characterization of biodegradable nanoparticles based on poly (γ-glutamic acid) with L-phenylalanine as a protein carrier. J Control Release 108(2-3):226–236. https://doi.org/10.1016/j.jconrel.2005.08.003
Hoennscheidt C, Kreyenschulte D, Margaritis A, Krull R (2013) Production of stable quinine nanodispersions using esterified γ-polyglutamic acid biopolymer. Biochem Eng J 79:259–266. https://doi.org/10.1016/j.bej.2013.08.004
Zanuy D, Alemán C (2007) Molecular dynamics study of complexes of poly (glutamate) and dodecyltrimethylammonium. Biomacromolecules 8(2):663–671. https://doi.org/10.1021/bm060927c
Ponomarenko EA, Waddon AJ, Bakeev KN, Tirrell DA, MacKnight WJ (1996) Self-assembled complexes of synthetic polypeptides and oppositely charged low molecular weight surfactants. Solid-state properties. Macromolecules 29(12):4340–4345. https://doi.org/10.1021/ma951088h
Han TH, Ok T, Kim J, Shin DO, Ihee H, Lee HS, Kim SO (2010) Bionanosphere lithography via hierarchical peptide self-assembly of aromatic triphenylalanine. Small 6(8):945–951. https://doi.org/10.1002/smll.200902050
Liu F, Huang X, Han L, Sang M, Hu L, Liu B, Duan B, Jiang P, Wang X, Qiao Z, Ma C (2019) Improved druggability of gambogic acid using core–shell nanoparticles. Biomater Sci 7(3):1028–1042. https://doi.org/10.1039/C8BM01154K
Ashiuchi M, Tani K, Soda K, Misono H (1998) Properties of glutamate racemase from Bacillus subtilis IFO 3336 producing poly-γ- glutamate. J Biochem 123(6):1156–1163. https://doi.org/10.1093/oxfordjournals.jbchem.a022055
Ashiuchi M, Soda K, Misono H (1999b) A poly-γ-glutamate synthetic system of Bacillus subtilis IFO 3336: gene cloning and biochemical analysis of poly-γ-glutamate produced by Escherichia coli clone cells. Biochem Biophys Res Commun 263(1):6–12. https://doi.org/10.1006/bbrc.1999.1298
Kada S, Nanamiya H, Kawamura F, Horinouchi S (2004) Glr, a glutamate racemase, supplies D-glutamate to both peptidoglycan synthesis and poly-γ-glutamate production in γ-PGA-producing Bacillus subtilis. FEMS Microbiol Lett 236(1):13–20. https://doi.org/10.1016/j.femsle.2004.05.028
Sung MH, Park C, Kim CJ, Poo H, Soda K, Ashiuchi M (2005b) Natural and edible biopolymer poly-γ-glutamic acid: synthesis, production, and applications. Chem Rec 5(6):352–366. https://doi.org/10.1002/tcr.20061
Tran LS, Nagai T, Itoh Y (2000) Divergent structure of the ComQXPA quorum-sensing components: molecular basis of strain-specific communication mechanism in Bacillus subtilis. Mol Microbiol 37(5):1159–1171. https://doi.org/10.1046/j.1365-2958.2000.02069.x
Stanley NR, Lazazzera BA (2005) Defining the genetic differences between wild and domestic strains of Bacillus subtilis that affect poly-γ-DL-glutamic acid production and biofilm formation. Mol Microbiol 57(4):1143–1158. https://doi.org/10.1111/j.1365-2958.2005.04746.x
Obst M, Steinbüchel A (2004) Microbial degradation of poly (amino acid) s. Biomacromolecules 5(4):1166–1176. https://doi.org/10.1021/bm049949u
Odeniyi O, Avoseh D (2018) Effects of media components and agricultural by-products on γ-polyglutamic acid production by Bacillus toyonensis As8. Polim Med 48(2):91–97. https://doi.org/10.17219/pim/105555
Fang J, Huan C, Liu Y, Xu L, Yan Z (2020) Bioconversion of agricultural waste into poly-γ-glutamic acid in solid-state bioreactors at different scales. Waste Manag 102:939–948. https://doi.org/10.1016/j.wasman.2019.12.016
Mohanraj R, Gnanamangai BM, Ramesh K, Priya P, Srisunmathi R, Poornima S, Ponmurugan P, Robinson JP (2019) Optimized production of gamma poly glutamic acid (γ-PGA) using sago. Biocatal Agric Biotechnol 22:101413. https://doi.org/10.1016/j.bcab.2019.101413
Zhang C, Wu DJ, Jia J, Yang HQ (2019) Fishmeal wastewater as a low-cost nitrogen source for γ-polyglutamic acid production using Bacillus subtilis. Waste Biomass Valorization 10(4):789–795. https://doi.org/10.1007/s12649-017-0100-1
Birrer GA, Cromwick AM, Gross RA (1994) γ-Poly(glutamic acid) formation by Bacillus licheniformis 9945a: physiological and biochemical studies. Int J Biol Macromol 16(5):265–275. https://doi.org/10.1016/0141-8130(94)90032-9
Bajaj IB, Lele SS, Singhal RS (2009) A statistical approach to optimization of fermentative production of poly (γ-glutamic acid) from Bacillus licheniformis NCIM 2324. Bioresour Technol 100(2):826–832. https://doi.org/10.1016/j.biortech.2008.06.047
Bajaj IB, Singhal RS (2009) Enhanced production of poly (γ-glutamic acid) from Bacillus licheniformis NCIM 2324 by using metabolic precursors. Appl Biochem Biotechnol 159(1):133–141. https://doi.org/10.1007/s12010-008-8427-5
Mabrouk M, Abou-Zeid D, Sabra W (2012) Application of Plackett–Burman experimental design to evaluate nutritional requirements for poly(γ-glutamic acid) production in batch fermentation by Bacillus licheniformis A13. Afr J Appl Microb Res 1:6–18
Huang J, Du Y, Xu G, Zhang H, Zhu F, Huang L, Xu Z (2011) High yield and cost-effective production of poly (γ-glutamic acid) with Bacillus subtilis. Eng Life Sci 11(3):291–297. https://doi.org/10.1002/elsc.201000133
Zhang C, Wu D, Qiu X (2018) Stimulatory effects of amino acids on γ-polyglutamic acid production by Bacillus subtilis. Sci Rep 8(1):1–9
Ji XJ, Nie ZK, Huang H, Ren LJ, Peng C, Ouyang PK (2011) Elimination of carbon catabolite repression in Klebsiella oxytoca for efficient 2, 3-butanediol production from glucose–xylose mixtures. Appl Microbiol Biotechnol 89(4):1119–1125. https://doi.org/10.1007/s00253-010-2940-5
Cromwick AM, Birrer GA, Gross RA (1996) Effects of pH and aeration on γ-poly (glutamic acid) formation by Bacillus licheniformis in controlled batch fermentor cultures. Biotechnol Bioeng 50(2):222–227. https://doi.org/10.1002/(SICI)1097-0290(19960420)50:2<222::AID-BIT10>3.0.CO;2-P
Richard A, Margaritis A (2003) Optimization of cell growth and poly (glutamic acid) production in batch fermentation by Bacillus subtilis. Biotechnol Lett 25(6):465–468. https://doi.org/10.1023/A:1022644417429
Wu Q, Xu H, Ying H, Ouyang P (2010) Kinetic analysis and pH-shift control strategy for poly (γ-glutamic acid) production with Bacillus subtilis CGMCC 0833. Biochem Eng J 50(1-2):24–28. https://doi.org/10.1016/j.bej.2010.02.012
Xu Z, Shi F, Cen P (2005) Production of polyglutamic acid from mixed glucose and sucrose by co-cultivation of Bacillus subtilis and Corynebacterium glutamicum. In: The 2005 AIChE annual meeting, Cincinnati, 4 November 2005
Do JH, Chang HN, Lee SY (2001) Efficient recovery of gamma-poly (glutamic acid) from highly viscous culture broth. Biotechnol Bioeng 76(3):219–223. https://doi.org/10.1002/bit.1186
Park C, Choi JC, Choi YH, Nakamura H, Shimanouchi K, Horiuchi T, Misono H, Sewaki T, Soda K, Ashiuchi M, Sung MH (2005) Synthesis of super-high-molecular-weight poly-γ-glutamic acid by Bacillus subtilis subsp. chungkookjang. J Mol Catal B Enzym 35(4-6):128–133. https://doi.org/10.1016/j.molcatb.2005.06.007
McLean RJ, Beauchemin D, Clapham L, Beveridge TJ (1990) Metal-binding characteristics of the gamma-glutamyl capsular polymer of Bacillus licheniformis ATCC 9945. Appl Environ Microbiol 56(12):3671–3677. https://doi.org/10.1128/aem.56.12.3671-3677.1990
Yokoi H, Natsuda O, Hirose J, Hayashi S, Takasaki Y (1995) Characteristics of a biopolymer flocculant produced by Bacillus sp. PY-90. J Ferment Bioeng 79(4):378–380. https://doi.org/10.1016/0922-338X(95)94000-H
Goto A, Kunioka M (1992) Biosynthesis and hydrolysis of poly (γ-glutamic acid) from Bacillus subtilis IF03335. Biosci Biotechnol Biochem 56(7):1031–1035. https://doi.org/10.1271/bbb.56.1031
Luo Z, Guo Y, Liu J, Qiu H, Zhao M, Zou W, Li S (2016) Microbial synthesis of poly-γ-glutamic acid: current progress, challenges, and future perspectives. Biotechnol Biofuels 9(1):1–12
Khalil IR, Burns AT, Radecka I, Kowalczuk M, Khalaf T, Adamus G, Johnson B, Khechara MP (2017) Bacterial-derived polymer poly-γ-glutamic acid (γ-PGA)-based micro/nanoparticles as a delivery system for antimicrobials and other biomedical applications. Int J Mol Sci 18(2):313. https://doi.org/10.3390/ijms18020313
Ourique AF, Pohlmann AR, Guterres SS, Beck RCR (2008) Tretinoin-loaded nanocapsules: preparation, physicochemical characterization, and photostability study. Int J Pharm 352(1-2):1–4. https://doi.org/10.1016/j.ijpharm.2007.12.035
Shekhar K, Madhu MN, Pradeep B, Banji D (2010) A review on microencapsulation. Int J Pharm Sci Rev Res 5:58–62
Soppinath KS, Aminabhavi TM, Kulkurni AR, Rudzinski WE (2001) Biodegradable polymeric nanoparticles as drug delivery devices. J Control Release 70(1-2):1–20. https://doi.org/10.1016/S0168-3659(00)00339-4
Owens DE III, Peppas NA (2006) Opsonization, biodistribution, and pharmacokinetics of polymeric nanoparticles. Int J Pharm 307(1):93–102. https://doi.org/10.1016/j.ijpharm.2005.10.010
Manocha B, Margaritis A (2008) Production and characterization of γ-polyglutamic acid nanoparticles for controlled anticancer drug release. Crit Rev Biotechnol 28(2):83–99. https://doi.org/10.1080/07388550802107483
Matsusaki M, Hiwatari KI, Higashi M, Kaneko T, Akashi M (2004) Stably dispersed and surface-functional bionanoparticles prepared u self-assembling amphipathic polymers of hydrophilic poly(γ-glutamic acid) bearing hydrophobic amino acids. Chem Lett 33(4):398–399. https://doi.org/10.1246/cl.2004.398
Muller M, Reihs T, Ouyang W (2005) Needle-like and spherical polyelectrolyte complex nanoparticles of poly(L-lysine) and copolymers of maleic acid. Langmuir 21(1):465–469. https://doi.org/10.1021/la0483257
Das MK, Sarma A, Chakraborty T (2016) PLGA-derived anticancer nano therapeutics: Promises and challenges for the future. J Chem Pharm Res 8(2):484–499
Redhead HM, Davis SS, Illum L (2001) Drug delivery in poly (lactide-co-glycolide) nanoparticles surface modified with poloxamer 407 and poloxamine 908: in vitro characterisation and in vivo evaluation. J Control Release 70(3):353–363. https://doi.org/10.1016/S0168-3659(00)00367-9
Shang L, Nienhaus K, Nienhaus GU (2014) Engineered nanoparticles interacting with cells: size matters. J Nanobiotechnology 12(1):1–11
Rice SB, Chan C, Brown SC, Eschbach P, Han L, Ensor DS, Stefaniak AB, Bonevich J, Vladár AE, Walker ARH, Zheng J (2013) Particle size distributions by transmission electron microscopy: An interlaboratory comparison case study. Metrologia 50(6):663–678. https://doi.org/10.1088/0026-1394/50/6/663
Pal SL, Jana U, Manna PK, Mohanta GP, Manavalan R (2011) Nanoparticle: an overview of preparation and characterization. J Appl Pharm Sci 1(6):228–234
Su Z, Han C, Liu E, Zhang F, Liu B, Meng X (2021) Formation, characterization and application of arginine-modified chitosan/γ-poly glutamic acid nanoparticles as carrier for curcumin. Int J Biol Macromol 168:215–222. https://doi.org/10.1016/j.ijbiomac.2020.12.050
Singer JW (2005) Paclitaxel poliglumex (XYOTAX, CT-2103): a macromolecular taxane. J Control Release 109(1-3):120–126. https://doi.org/10.1016/j.jconrel.2005.09.033
Ye H, Jin L, Hu R, Yi Z, Li J, Wu Y, Xi X, Wu Z (2006) Poly (γ, l-glutamic acid)–cisplatin conjugate effectively inhibits human breast tumor xenografted in nude mice. Biomaterials 27(35):5958–5965. https://doi.org/10.1016/j.biomaterials.2006.08.016
Liu B, Che C, Liu J, Si M, Gong Z, Li Y, Zhang J, Yang G (2019) Fabrication and antitumor mechanism of a nanoparticle drug delivery system: graphene oxide/chitosan oligosaccharide/γ-Polyglutamic acid composites for anticancer drug delivery. ChemistrySelect 4(43):12491–12502. https://doi.org/10.1002/slct.201903145
Zia Q, Khan AA, Swaleha Z, Owais M (2015) Self-assembled amphotericin B-loaded polyglutamic acid nanoparticles: preparation, characterization and in vitro potential against Candida albicans. Int J Nanomedicine 10:1769–1790. https://doi.org/10.2147/IJN.S63155
Sonaje K, Chen YJ, Chen HL, Wey SP, Juang JH, Nguyen HN, Hsu CW, Lin KJ, Sung HW (2010) Enteric-coated capsules filled with freeze-dried chitosan/poly (γ-glutamic acid) nanoparticles for oral insulin delivery. Biomaterials 31(12):3384–3394. https://doi.org/10.1016/j.biomaterials.2010.01.042
Carino GP, Mathiowitz E (1999) Oral insulin delivery. Adv Drug Deliv Rev 35(2-3):249–257. https://doi.org/10.1016/S0169-409X(98)00075-1
Zambanini A, Newson RB, Maisey M, Feher MD (1999) Injection related anxiety in insulin-treated diabetes. Diabetes Res Clin Pract 46(3):239–246. https://doi.org/10.1016/S0168-8227(99)00099-6
Lin YH, Sonaje K, Lin KM, Juang JH, Mi FL, Yang HW, Sung HW (2008) Multi-ion-crosslinked nanoparticles with pH-responsive characteristics for oral delivery of protein drugs. J Control Release 132(2):141–149. https://doi.org/10.1016/j.jconrel.2008.08.020
No funding received
Ethics approval and consent to participate
Consent for publication
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Balogun-Agbaje, O.A., Odeniyi, O.A. & Odeniyi, M.A. Drug delivery applications of poly-γ-glutamic acid. Futur J Pharm Sci 7, 125 (2021). https://doi.org/10.1186/s43094-021-00280-w
- Poly-γ-glutamic acid
- Medium optimization
- Drug delivery